Equilib Cooling Calculations

# Equilib Cooling Calculations

## Equilib Cooling Calculations

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -
##### Presentation Transcript

1. EquilibCooling Calculations • The Equilib module enables you to perform cooling calculations and display the phase transitions and compositions during • Equilibrium cooling • Scheil-Gulliver cooling • Full annealing of cast alloys Table of Contents Section 13.1 Table of Contents Section 13.2Phase transitions : FeO-MnO Section 13.3Simple equilibrium cooling : FeO-MnO Section 13.4Simple Scheil-Gulliver cooling : FeO-MnO Section 13.5Equilibrium cooling, plots: Al-Mg-Zn Section 13.6Scheil-Gulliver cooling, plots : Al-Mg-Zn Section 13.7Scheil-Gulliver cooling, annealing casted alloy : Al-Mg-Zn-Mn Section 13.8 Scheil-Gulliver cooling, plots: gas phase Equilib Cooling Calculations 13.1

2. FeO-MnO : Phase transitions - binary phase diagram <A> = XMnO =0.5 Tliquidus = 1620.23°C Tsolidus = 1529.1°C FeO-MnO binary phase diagram calculated by Phase Diagram TFeO(melting point) = 1370.91°C Equilib Cooling Calculations 2.1

3. FeO-MnO :Equilibrium phase transitions at XFeO = 0.5 1° Binary system <1-A> MnO + <A> FeO . • 2° Possible products: • solid solution (MONO) • liquid Slag (SLAG) 3° <A> = 0.5T (°C) = 1500 and 1700 Equilibwillcalculate the equilibriumatXFeO = 0.5 for temperaturesvaryingfrom1500°C to 1700°C and willsearch for All phase transitions. Equilib Cooling Calculations 2.2

4. FeO-MnO :Phase transitionsshowing liquidus and solidus Equilibrium solidus Equilibrium liquidus Equilib Cooling Calculations 2.3

5. FeO-MnO :Simple equilibium cooling – L-Option 1° Right-click on the ‘+’ column to open the SLAG extended menu and selectL– cooLing calculation.to open the Cooling Calculation Window • 2° Cooling Calculation Window • selectequilibrium cooling • check√ transitions + summary • clickOKto close. Equilib Cooling Calculations 3.1

6. FeO-MnO :Simple equilibium cooling – step, T-auto and stop • EquilibriumCoolingof SLAG • coolingstep ‘5’ (0.1 – 250) • T-auto√ automatically • calculates the starting T • final mass ‘0’ (i.e. stops after • complete solidification) In equilibrium cooling the cooling step (’5’) defines the pages displayed in the Results Window. (i.e. every 5 degrees). The cooling step has no effect on the transitions or when 100% solidification is attained. Enter default starting temperature ‘1650’ – applied when T-auto is not used Equilib Cooling Calculations 3.2

7. FeO-MnO :Equilibrium cooling – Summaryand Transitions Summary Transitions Equilib Cooling Calculations 3.3

8. FeO-MnO :Equilibrium cooling - Liquidus and Solidus Liquidus Solidus Equilib Cooling Calculations 3.4

9. Scheil target phase The program performs a Gulliver-Scheil cooling calculation. That is, as phases precipitate from the Scheil target phase they are dropped from the total mass balance. Generally a value of T (the initial temperature) and a cooling step must be specified in the Final Conditions frame. Normally, the Scheil calculation is repeated until the Scheil Target phase disappears. However it is possible to stop the calculation by either specifying a second temperature in the Final Conditions frame, or by specifying a target mass. The Scheil target phase must be the gas phase or a real solution. If it is a liquid phase (such as FToxid-SLAG and Ftsalt-liquid) then the precipitates are generally solids - it would be unusual in this case to select and include other liquids or the gas phase in the calculation. If the Scheil target phase is the gas phase then the precipitates could be any or all of the other compound and solution phases. To activate a Scheil target gas phase, first select the gas species in the usual way. Then with the mouse-right-button click on the gas '+' check box in the compound species frame of the Menu Window - this will open the Species Selection window. Point to the '+' column of any selected gas species and then click with the mouse-right-button and then select «Scheil cooling gas phase». Equilib Cooling Calculations

10. FeO-MnO :Scheil-Gulliver cooling – L-Option 1° Right-click on the ‘+’ column to open the FACT-SLAG extended menu and selectL– cooLing calculation.to open the Cooling Calculation Window • 2° Cooling Calculation Window • selectScheil-Gulliver cooling • check√ transitions + summary. • clickOKto close. Equilib Cooling Calculations 4.1

11. FeO-MnO :Scheil-Gulliver cooling – step, T-auto and stop In Scheil-Gulliver cooling the cooling step (’5’) defines the calculation step (i.e. every 5 degrees). After each calculation any phase that precipitates from the solution phase is dropped from the total mass balance. The size of the step effects the calculated results. The smaller the step, the more precise the calculation and the longer the calculation time. • Scheil-Gulliver Coolingof SLAG • coolingstep ‘5’ (0.1 – 250) • T-auto√ automatically • calculates the starting T • final mass ‘0’ (i.e. stops after • complete solidification) Enter default starting temperature ‘1650’ – this is applied when T-auto is not used Equilib Cooling Calculations 4.2

12. FeO-MnO :Scheil cooling – Summaryand Transitions Summary Transitions Equilib Cooling Calculations 4.3

13. FeO-MnO :Scheil cooling – Startand Stop Start of solidification at 1620.23oC End of solidification at 1376.68oC The size of the cooling step effects the calculated results. Here the step 5oC gives 1376.68oC. The end of Scheil solidification should be at 1370.91oC – the melting point of FeO. With a much smaller step, 0.1oC, one obtains ~ 1370.9oC.. Equilib Cooling Calculations 4.4

14. FeO-MnO :Scheil cooling – incremental vs.accumulated Incremental Scheil solidification at 1500oC Accumulated Scheil solidification at 1500oC Equilib Cooling Calculations 4.5

15. Al-Mg-Zn :Equilibrium cooling XMg=0.8,XAl=0.15,XZn=0.05 Al-Mg-Znpolythermalliquidus projection calculated by Phase Diagram with data taken from FTlite – FACT light alloy databases Equilib Cooling Calculations 5.1

16. Al-Mg-Zn :Equilibium cooling – L-Option • EquilibriumCooling • of Liquid Al-Mg-Zn • coolingstep ‘10’ • T-auto √ • final mass ‘0’ Equilib Cooling Calculations 5.2

17. Al-Mg-Zn :Equilibium cooling – Summary of Results Equilib Cooling Calculations 5.3

18. Al-Mg-Zn :Equilibium cooling – Plot Results Equilib Cooling Calculations 5.4

19. Al-Mg-Zn :Equilibium cooling – Plot Results Selection of species to be plotted (choose all solids and elements for which Gram(Max)>0) Equilib Cooling Calculations 5.5

20. Al-Mg-Zn :Equilibium cooling – Plot Results Liquidus at about 500 oC Univariant at about 400 oC ??? reaction at about 300 oC Equilib Cooling Calculations 5.6

21. Al-Mg-Zn :Scheil cooling XMg=0.8,XAl=0.15,XZn=0.05 Al-Mg-Znpolythermalliquidus projection calculated by Phase Diagram with data taken from FTlite – FACT light alloy databases Equilib Cooling Calculations 6.1

22. Al-Mg-Zn :Scheil-Gulliver cooling – L-Option • ScheilCooling • of Liquid Al-Mg-Zn • coolingstep ‘10’ • check T-auto √ • enter final mass ‘0’ Equilib Cooling Calculations 6.2

23. Graphical output of Scheil target calculation - Calculation ends at temperature of final disappearance of liquid - Graph shows phase distribution Equilib Cooling Calculations 6.3

24. Al-Mg-Zn-Mn :Scheil cooling AZ91 + 0.25 wt.% Mn alloy • ScheilCooling • of Liquid Al-Mg-Zn-Mn • coolingstep ‘10’ • check T-auto √ • enter final mass ‘0’ Equilib Cooling Calculations 6.4

25. Al-Mg-Zn-Mn :Scheil cooling – Summaryand Transitions AZ91 + 0.25 wt.% Mn alloy: 89.75Al-9Mg-Zn-0.25Mg (wt%) Summary Transitions Equilib Cooling Calculations 6.5

26. Al-Mg-Zn-Mn :Scheil cooling - Microstructure Constituents Summary & TransitionsMicrostructure constituents of AZ91 + 0.25 wt.% Mn alloy after Scheil cooling. Final disappearance of liquid at 340.89°C Equilib Cooling Calculations 7.6

27. CONS. PHASE TOTAL AMT/gram 1 1 ‘Al8Mn5’ 5.2241E-04 2 1 HCP 6.4599E+01 2 2 ‘Al8Mn5’ 2.8231E-01 3 1 HCP 1.5644E+01 3 2 Al11Mn4 1.4638E-01 4 1 HCP 1.7084E+00 4 2 ‘Al4Mn’ 1.7892E-02 5 1 HCP 4.9213E+00 5 2 ‘Al12Mg17’1.1878E+01 5 3 ‘Al4Mn’ 2.6558E-02 6 1 HCP 1.9669E-01 6 2 Phi 4.0423E-01 6 3 ‘Al4Mn’ 1.7904E-05 6 4 Al11Mn4 3.8196E-05 7 1 HCP 2.4177E-02 7 2 Tau 3.5706E-02 7 3 Al11Mn4 1.4894E-06 8 1 HCP 4.2084E-02 8 2 MgZn 5.1501E-02 8 3 Tau 2.1364E-02 8 4 Al11Mn4 2.3786E-06 Tracking microstructure constituents Output : Solidification temperature of 340.89°C Amount & Average Composition of the HCP phase • Solidification software (extended Scheil cooling) • Scheil cooling + post equilibration (annealing) of Scheil microstructure • AZ91 alloy + 0.25 wt.% Mn Equilib Cooling Calculations 7.7

28. Al-Mg-Zn-Mn : Selecting constituent 2 HCP phase for annealing 1° Point mouse to constituent 2HCP_A3 and double-click 2° Click OK to recycle HCP_A3 Equilib Cooling Calculations 7.1

29. Al-Mg-Zn-Mn : HCP phase imported into Reactant Window Change mass from 100% => 100 g List of components in HCP phase Equilib Cooling Calculations 7.2

30. Al-Mg-Zn-Mn : Equilibrium calculation – annealing HCP phase Anneal at 150 to 500 oC Equilib Cooling Calculations 7.3

31. Al-Mg-Zn-Mn : Plotting annealed HCP phase Equilib Cooling Calculations 7.4

32. Al-Mg-Zn-Mn : Graph of annealed HCP phase Equilibrium phase distribution in HCP phase of constituent 2 after annealing (HCP + precipitates) Equilib Cooling Calculations 7.5

33. Equilibrium phase distribution in HCP phase of constituent 2 after annealing (HCP + precipitates) Equilib Cooling Calculations 7.6

34. Tracking microstructure constituents Annealing Phases vs T for HCP in the different microstructural constituents Annealing of HCP in ‘2’ Amount & Average Composition of the HCP phase at 340.89oC Annealing of HCP in ‘3’ • Solidification software (extended Scheil cooling) • Scheil cooling + post equilibration of Scheil microstructure • AZ91 alloy + 0.25 wt.% Mn Equilib Cooling Calculations